Further Reading 95Problems 954 Fluid Flow and Metal Evaporation in Welding 974.1 Fluid Flow in Arcs 974.2 Fluid Flow in Weld Pools 1034.3 Metal Evaporation 1144.4 Active Flux GTAW 116References 117Further Reading 119Problems 1205 Residual Stresses, Distortion, and Fatigue 1225.1 Residual Stresses 1225.2 Distortion 1265.3 Fatigue 1315.4 Case Studies 137References 140Further Reading 141Problems 141II THE FUSION ZONE 1436 Basic Solidiﬁcation Concepts 1456.1 Solute Redistribution during Solidiﬁcation 1456.2 Solidiﬁcation Modes and Constitutional Supercooling 1556.3 Microsegregation and Banding 1606.4 Effect of Cooling Rate 1636.5 Solidiﬁcation Path 166References 167Further Reading 168Problems 1697 Weld Metal Solidiﬁcation I: Grain Structure 1707.1 Epitaxial Growth at Fusion Boundary 1707.2 Nonepitaxial Growth at Fusion Boundary 1727.3 Competitive Growth in Bulk Fusion Zone 1747.4 Effect of Welding Parameters on Grain Structure 1747.5 Weld Metal Nucleation Mechanisms 1787.6 Grain Structure Control 187viii CONTENTS
References 195Further Reading 197Problems 1978 Weld Metal Solidiﬁcation II: Microstructure within Grains 1998.1 Solidiﬁcation Modes 1998.2 Dendrite and Cell Spacing 2048.3 Effect of Welding Parameters 2068.4 Reﬁning Microstructure within Grains 209References 213Further Reading 213Problems 2149 Post-Solidiﬁcation Phase Transformations 2169.1 Ferrite-to-Austenite Transformation in Austenitic StainlessSteel Welds 2169.2 Austenite-to-Ferrite Transformation in Low-Carbon,Low-Alloy Steel Welds 232References 239Further Reading 241Problems 24110 Weld Metal Chemical Inhomogeneities 24310.1 Microsegregation 24310.2 Banding 24910.3 Inclusions and Gas Porosity 25010.4 Inhomogeneities Near Fusion Boundary 25210.5 Macrosegregation in Bulk Weld Metal 255References 260Further Reading 261Problems 26111 Weld Metal Solidiﬁcation Cracking 26311.1 Characteristics, Cause, and Testing 26311.2 Metallurgical Factors 26811.3 Mechanical Factors 28411.4 Reducing Solidiﬁcation Cracking 28511.5 Case Study: Failure of a Large Exhaust Fan 295References 296Further Reading 299Problems 299CONTENTS ix
III THE PARTIALLY MELTED ZONE 30112 Formation of the Partially Melted Zone 30312.1 Evidence of Liquation 30312.2 Liquation Mechanisms 30412.3 Directional Solidiﬁcation of Liquated Material 31412.4 Grain Boundary Segregation 31412.5 Grain Boundary Solidiﬁcation Modes 31612.6 Partially Melted Zone in Cast Irons 318References 318Problems 31913 Difﬁculties Associated with the Partially Melted Zone 32113.1 Liquation Cracking 32113.2 Loss of Strength and Ductility 32813.3 Hydrogen Cracking 32813.4 Remedies 330References 336Problems 338IV THE HEAT-AFFECTED ZONE 34114 Work-Hardened Materials 34314.1 Background 34314.2 Recrystallization and Grain Growth in Welding 34714.3 Effect of Welding Parameters and Process 349References 351Further Reading 352Problems 35215 Precipitation-Hardening Materials I: Aluminum Alloys 35315.1 Background 35315.2 Al–Cu–Mg and Al–Mg–Si Alloys 35915.3 Al–Zn–Mg Alloys 36715.4 Friction Stir Welding of Aluminum Alloys 370References 371Further Reading 372Problems 37216 Precipitation-Hardening Materials II: Nickel-Base Alloys 37516.1 Background 375x CONTENTS
16.2 Reversion of Precipitate and Loss of Strength 37916.3 Postweld Heat Treatment Cracking 384References 390Further Reading 392Problems 39217 Transformation-Hardening Materials: Carbon andAlloy Steels 39317.1 Phase Diagram and CCT Diagrams 39317.2 Carbon Steels 39617.3 Low-Alloy Steels 40417.4 Hydrogen Cracking 41017.5 Reheat Cracking 41817.6 Lamellar Tearing 42217.7 Case Studies 425References 427Further Reading 429Problems 43018 Corrosion-Resistant Materials: Stainless Steels 43118.1 Classiﬁcation of Stainless Steels 43118.2 Austenitic Stainless Steels 43318.3 Ferritic Stainless Steels 44618.4 Martensitic Stainless Steels 44918.5 Case Study: Failure of a Pipe 451References 452Further Reading 453Problems 454Index 455CONTENTS xi
PREFACESince the publication of the ﬁrst edition of this book in 1987, there has beenmuch new progress made in welding metallurgy. The purpose for the secondedition is to update and improve the ﬁrst edition. Examples of improvementsinclude (1) much sharper photomicrographs and line drawings; (2) integrationof the phase diagram, thermal cycles, and kinetics with the microstructure toexplain microstructural development and defect formation in welds; and (3)additional exercise problems. Speciﬁc revisions are as follows.In Chapter 1 the illustrations for all welding processes have been re-drawn to show both the overall process and the welding area. In Chapter2 the heat source efﬁciency has been updated and the melting efﬁciencyadded. Chapter 3 has been revised extensively, with the dissolution ofatomic nitrogen, oxygen, and hydrogen in the molten metal considered andelectrochemical reactions added. Chapter 4 has also been revised extensively,with the arc added, and with ﬂow visualization, arc plasma dragging, andturbulence included in weld pool convection. Shot peening is added toChapter 5.Chapter 6 has been revised extensively, with solute redistribution andmicrosegregation expanded and the solidiﬁcation path added. Chapter 7 nowincludes nonepitaxial growth at the fusion boundary and formation of non-dendritic equiaxed grains. In Chapter 8 solidiﬁcation modes are explained withmore illustrations. Chapter 9 has been expanded signiﬁcantly to add ferriteformation mechanisms, new ferrite prediction methods, the effect of coolingrate, and factors affecting the austenite–ferrite transformation. Chapter 10now includes the effect of both solid-state diffusion and dendrite tip under-cooling on microsegregation. Chapter 11 has been revised extensively toinclude the effect of eutectic reactions, liquid distribution, and ductility ofthe solidifying metal on solidiﬁcation cracking and the calculation of fractionof liquid in multicomponent alloys.Chapter 12 has been rewritten completely to include six different liquationmechanisms in the partially melted zone (PMZ), the direction and modes ofgrain boundary (GB) solidiﬁcation, and the resultant GB segregation. Chapter13 has been revised extensively to include the mechanism of PMZ crackingand the effect of the weld-metal composition on cracking.Chapter 15 now includes the heat-affected zone (HAZ) in aluminum–lithium–copper welds and friction stir welds and Chapter 16 the HAZ ofInconel 718. Chapter 17 now includes the effect of multiple-pass welding onxiii
reheat cracking and Chapter 18 the grain boundary chromium depletion in asensitized austenitic stainless steel.The author thanks the National Science Foundation and NASA forsupporting his welding research, from which this book draws frequently.He also thanks the American Welding Society and ASM International for per-missions to use numerous copyrighted materials. Finally, he thanks C. Huang,G. Cao, C. Limmaneevichitr, H. D. Lu, K.W. Keehn, and T.Tantanawat for pro-viding technical material, requesting permissions, and proofreading.Sindo KouMadison, Wisconsinxiv PREFACE
PART IIntroductionWelding Metallurgy, Second Edition. Sindo KouCopyright 2003 John Wiley & Sons, Inc.ISBN: 0-471-43491-4
1 Fusion Welding ProcessesFusion welding processes will be described in this chapter, including gaswelding, arc welding, and high-energy beam welding. The advantages and dis-advantages of each process will be discussed.1.1 OVERVIEW1.1.1 Fusion Welding ProcessesFusion welding is a joining process that uses fusion of the base metal to makethe weld. The three major types of fusion welding processes are as follows:1. Gas welding:Oxyacetylene welding (OAW)2. Arc welding:Shielded metal arc welding (SMAW)Gas–tungsten arc welding (GTAW)Plasma arc welding (PAW)Gas–metal arc welding (GMAW)Flux-cored arc welding (FCAW)Submerged arc welding (SAW)Electroslag welding (ESW)3. High-energy beam welding:Electron beam welding (EBW)Laser beam welding (LBW)Since there is no arc involved in the electroslag welding process, it is notexactly an arc welding process. For convenience of discussion, it is groupedwith arc welding processes.1.1.2 Power Density of Heat SourceConsider directing a 1.5-kW hair drier very closely to a 304 stainless steel sheet1.6mm (1/16 in.) thick. Obviously, the power spreads out over an area of roughly3Welding Metallurgy, Second Edition. Sindo KouCopyright 2003 John Wiley & Sons, Inc.ISBN: 0-471-43491-4
50mm (2in.) diameter, and the sheet just heats up gradually but will not melt.With GTAW at 1.5kW, however, the arc concentrates on a small area of about6mm (1/4 in.) diameter and can easily produce a weld pool.This example clearlydemonstrates the importance of the power density of the heat source inwelding.The heat sources for the gas, arc, and high-energy beam welding processesare a gas ﬂame, an electric arc, and a high-energy beam, respectively. Thepower density increases from a gas ﬂame to an electric arc and a high-energybeam. As shown in Figure 1.1, as the power density of the heat sourceincreases, the heat input to the workpiece that is required for weldingdecreases.The portion of the workpiece material exposed to a gas ﬂame heatsup so slowly that, before any melting occurs, a large amount of heat is alreadyconducted away into the bulk of the workpiece. Excessive heating can causedamage to the workpiece, including weakening and distortion. On the con-trary, the same material exposed to a sharply focused electron or laser beamcan melt or even vaporize to form a deep keyhole instantaneously, and beforemuch heat is conducted away into the bulk of the workpiece, welding is com-pleted (1).Therefore, the advantages of increasing the power density of the heatsource are deeper weld penetration, higher welding speeds, and better weldquality with less damage to the workpiece, as indicated in Figure 1.1. Figure1.2 shows that the weld strength (of aluminum alloys) increases as the heatinput per unit length of the weld per unit thickness of the workpiece decreases(2). Figure 1.3a shows that angular distortion is much smaller in EBW than in4 FUSION WELDING PROCESSESIncreasingdamage toworkpieceIncreasingpenetration,welding speed,weld quality,equipment costPower density of heat sourcehigh energybeam weldingarcweldinggasweldingHeatinputtoworkpieceFigure 1.1 Variation of heat input to the workpiece with power density of the heatsource.
GTAW (2). Unfortunately, as shown in Figure 1.3b, the costs of laser and elec-tron beam welding machines are very high (2).1.1.3 Welding Processes and MaterialsTable 1.1 summarizes the fusion welding processes recommended for carbonsteels, low-alloy steels, stainless steels, cast irons, nickel-base alloys, andOVERVIEW 55040305 10 50 100 500Heat input, kJ/in./in.Strength,ksi703950836022196061Figure 1.2 Variation of weld strength with heat input per unit length of weld per unitthickness of workpiece. Reprinted from Mendez and Eagar (2).Productivity, cm/sFlameArcLaserelectronbeamProductivity, inch of weld/sCapitalequipment,dollarsPowerdensity,W/m20.1 1 10 1000.04 0.4 4 40 400103105107103105107(b)tEBWGTAWWeld thickness t, mm0 20 40Distortionangledegree24680(a)ααFigure 1.3 Comparisons between welding processes: (a) angular distortion; (b) capitalequipment cost. Reprinted from Mendez and Eagar (2).
aluminum alloys (3). For one example, GMAW can be used for all the materi-als of almost all thickness ranges while GTAW is mostly for thinner workpieces.For another example, any arc welding process that requires the use of a ﬂux,such as SMAW, SAW, FCAW, and ESW, is not applicable to aluminum alloys.1.1.4 Types of Joints and Welding PositionsFigure 1.4 shows the basic weld joint designs in fusion welding: the butt, lap,T-, edge, and corner joints. Figure 1.5 shows the transverse cross section ofsome typical weld joint variations. The surface of the weld is called the face,the two junctions between the face and the workpiece surface are called thetoes, and the portion of the weld beyond the workpiece surface is called thereinforcement. Figure 1.6 shows four welding positions.1.2 OXYACETYLENE WELDING1.2.1 The ProcessGas welding is a welding process that melts and joins metals by heating themwith a ﬂame caused by the reaction between a fuel gas and oxygen. Oxy-acetylene welding (OAW), shown in Figure 1.7, is the most commonly usedgas welding process because of its high ﬂame temperature.A ﬂux may be usedto deoxidize and cleanse the weld metal. The ﬂux melts, solidiﬁes, and formsa slag skin on the resultant weld metal. Figure 1.8 shows three different typesof ﬂames in oxyacetylene welding: neutral, reducing, and oxidizing (4), whichare described next.1.2.2 Three Types of FlamesA. Neutral Flame This refers to the case where oxygen (O2) and acetylene(C2H2) are mixed in equal amounts and burned at the tip of the welding torch.A short inner cone and a longer outer envelope characterize a neutral ﬂameOXYACETYLENE WELDING 7(a) butt joint(c) T-joint(b) lap joint(d) edge joint(e) corner jointFigure 1.4 Five basic types of weld joint designs.
(Figure 1.8a). The inner cone is the area where the primary combustion takesplace through the chemical reaction between O2 and C2H2, as shown in Figure1.9. The heat of this reaction accounts for about two-thirds of the total heatgenerated.The products of the primary combustion, CO and H2, react with O2from the surrounding air and form CO2 and H2O. This is the secondary com-bustion, which accounts for about one-third of the total heat generated. Thearea where this secondary combustion takes place is called the outer enve-lope. It is also called the protection envelope since CO and H2 here consumethe O2 entering from the surrounding air, thereby protecting the weld metalfrom oxidation. For most metals, a neutral ﬂame is used.B. Reducing Flame When excess acetylene is used, the resulting ﬂame iscalled a reducing ﬂame.The combustion of acetylene is incomplete.As a result,a greenish acetylene feather between the inert cone and the outer envelopecharacterizes a reducing ﬂame (Figure 1.8b). This ﬂame is reducing in natureand is desirable for welding aluminum alloys because aluminum oxidizeseasily. It is also good for welding high-carbon steels (also called carburizingﬂame in this case) because excess oxygen can oxidize carbon and form CO gasporosity in the weld metal.8 FUSION WELDING PROCESSESToeToeReinforcementT-joint;fillet weldButt joint;square weldToeReinforcementButt joint;single-V-groove weldRootToeLap joint;fillet weldToeToe(d)(c)(a)(b)ToeT-joint;single bevel weldToe(e)Figure 1.5 Typical weld joint variations.
OXYACETYLENE WELDING 9(a) flat (b) horizontal(c) vertical (d) overheadFigure 1.6 Four welding positions.Oxygen/acetylenemixtureFiller rodProtectionenvelopeMetaldropletBase metal Weld poolWeldmetalSlagPrimarycombustionRegulatorFlow meterAcetyleneWeldingdirectionGas torchWorkpieceC2H2O2ValveOxygen(a)(b)Figure 1.7 Oxyacetylene welding: (a) overall process; (b) welding area enlarged.
C. Oxidizing Flame When excess oxygen is used, the ﬂame becomes oxi-dizing because of the presence of unconsumed oxygen. A short white innercone characterizes an oxidizing ﬂame (Figure 1.8c). This ﬂame is preferredwhen welding brass because copper oxide covers the weld pool and thus pre-vents zinc from evaporating from the weld pool.1.2.3 Advantages and DisadvantagesThe main advantage of the oxyacetylene welding process is that the equip-ment is simple, portable, and inexpensive.Therefore, it is convenient for main-tenance and repair applications. However, due to its limited power density, the10 FUSION WELDING PROCESSESinner coneinner coneacetylene featherReducing Flameinner cone Oxidizing FlameNeutral Flame(a)(b)(c)Figure 1.8 Three types of ﬂames in oxyacetylene welding. Modiﬁed from WeldingJournal (4). Courtesy of American Welding Society.C2H2 + O2GasTorch2500 oC1000 oC2800 - 3500 oCinnerconeouterenvelope2C2H2 + 2O2 (from cylinder)Secondary combustion in outerenvelope (1/3 total heat) :4CO + 2H24CO + 2O2 (from air) 4CO22H2 + O2 (from air) 2H2OPrimary combustion in innercone (2/3 total heat) :FlameFigure 1.9 Chemical reactions and temperature distribution in a neutral oxyacetyleneﬂame.
welding speed is very low and the total heat input per unit length of the weldis rather high, resulting in large heat-affected zones and severe distortion.Theoxyacetylene welding process is not recommended for welding reactive metalssuch as titanium and zirconium because of its limited protection power.1.3 SHIELDED METAL ARC WELDING1.3.1 The ProcessShielded metal arc welding (SMAW) is a process that melts and joins metalsby heating them with an arc established between a sticklike covered electrodeand the metals, as shown in Figure 1.10. It is often called stick welding.The electrode holder is connected through a welding cable to one terminalof the power source and the workpiece is connected through a second cableto the other terminal of the power source (Figure 1.10a).The core of the covered electrode, the core wire, conducts the electriccurrent to the arc and provides ﬁller metal for the joint. For electrical contact,the top 1.5cm of the core wire is bare and held by the electrode holder. Theelectrode holder is essentially a metal clamp with an electrically insulatedoutside shell for the welder to hold safely.The heat of the arc causes both the core wire and the ﬂux covering at theelectrode tip to melt off as droplets (Figure 1.10b). The molten metal collectsin the weld pool and solidiﬁes into the weld metal. The lighter molten ﬂux, onthe other hand, ﬂoats on the pool surface and solidiﬁes into a slag layer at thetop of the weld metal.1.3.2 Functions of Electrode CoveringThe covering of the electrode contains various chemicals and even metalpowder in order to perform one or more of the functions described below.A. Protection It provides a gaseous shield to protect the molten metal fromair. For a cellulose-type electrode, the covering contains cellulose, (C6H10O5)x.A large volume of gas mixture of H2, CO, H2O, and CO2 is produced whencellulose in the electrode covering is heated and decomposes. For a limestone-(CaCO3Ϫ) type electrode, on the other hand, CO2 gas and CaO slag form whenthe limestone decomposes. The limestone-type electrode is a low-hydrogen-type electrode because it produces a gaseous shield low in hydrogen. It is oftenused for welding metals that are susceptible to hydrogen cracking, such ashigh-strength steels.B. Deoxidation It provides deoxidizers and ﬂuxing agents to deoxidize andcleanse the weld metal. The solid slag formed also protects the already solid-iﬁed but still hot weld metal from oxidation.SHIELDED METAL ARC WELDING 11
C. Arc Stabilization It provides arc stabilizers to help maintain a stablearc. The arc is an ionic gas (a plasma) that conducts the electric current.Arc stabilizers are compounds that decompose readily into ions in the arc,such as potassium oxalate and lithium carbonate. They increase the electricalconductivity of the arc and help the arc conduct the electric current moresmoothly.D. Metal Addition It provides alloying elements and/or metal powder tothe weld pool. The former helps control the composition of the weld metalwhile the latter helps increase the deposition rate.1.3.3 Advantages and DisadvantagesThe welding equipment is relatively simple, portable, and inexpensive as com-pared to other arc welding processes. For this reason, SMAW is often used formaintenance, repair, and ﬁeld construction. However, the gas shield in SMAWis not clean enough for reactive metals such as aluminum and titanium. Thedeposition rate is limited by the fact that the electrode covering tends to over-heat and fall off when excessively high welding currents are used. The limitedlength of the electrode (about 35cm) requires electrode changing, and thisfurther reduces the overall production rate.12 FUSION WELDING PROCESSESGaseous shieldCore wireFlux coveringSlagMetaldropletFluxdropletBase metal Weld poolWeldmetalArc(a)(b)PowerSourceCable 1ElectrodeholderStickelectrodeWeldingdirectionWorkpieceCable 2Figure 1.10 Shielded metal arc welding: (a) overall process; (b) welding area enlarged.
1.4 GAS–TUNGSTEN ARC WELDING1.4.1 The ProcessGas–tungsten arc welding (GTAW) is a process that melts and joins metals byheating them with an arc established between a nonconsumable tungsten elec-trode and the metals, as shown in Figure 1.11. The torch holding the tungstenelectrode is connected to a shielding gas cylinder as well as one terminal ofthe power source, as shown in Figure 1.11a. The tungsten electrode is usuallyin contact with a water-cooled copper tube, called the contact tube, as shownin Figure 1.11b, which is connected to the welding cable (cable 1) from theterminal. This allows both the welding current from the power source toenter the electrode and the electrode to be cooled to prevent overheating.Theworkpiece is connected to the other terminal of the power source through adifferent cable (cable 2). The shielding gas goes through the torch body andis directed by a nozzle toward the weld pool to protect it from the air. Pro-tection from the air is much better in GTAW than in SMAW because an inertgas such as argon or helium is usually used as the shielding gas and becausethe shielding gas is directed toward the weld pool. For this reason, GTAW isGAS–TUNGSTEN ARC WELDING 13Shielding gasnozzleWeldmetalMetaldropletShieldinggasBase metal Weld poolArcFillerrodWeldingdirectionFiller rodTorchCable 1WorkpieceShieldinggascylinderFlowmeterRegulatorTungsten electrode(a)(b)PowersourceContact tubeShieldinggasCable 1Cable 2Figure 1.11 Gas–tungsten arc welding: (a) overall process; (b) welding area enlarged.
also called tungsten–inert gas (TIG) welding. However, in special occasions anoninert gas (Chapter 3) can be added in a small quantity to the shielding gas.Therefore, GTAW seems a more appropriate name for this welding process.When a ﬁller rod is needed, for instance, for joining thicker materials, it canbe fed either manually or automatically into the arc.1.4.2 PolarityFigure 1.12 shows three different polarities in GTAW (5), which are describednext.A. Direct-Current Electrode Negative (DCEN) This, also called the straightpolarity, is the most common polarity in GTAW.The electrode is connected tothe negative terminal of the power supply.As shown in Figure 1.12a, electronsare emitted from the tungsten electrode and accelerated while travelingthrough the arc. A signiﬁcant amount of energy, called the work function, isrequired for an electron to be emitted from the electrode. When the electronenters the workpiece, an amount of energy equivalent to the work function isreleased. This is why in GTAW with DCEN more power (about two-thirds) islocated at the work end of the arc and less (about one-third) at the electrodeend. Consequently, a relatively narrow and deep weld is produced.B. Direct-Current Electrode Positive (DCEP) This is also called the reversepolarity. The electrode is connected to the positive terminal of the powersource. As shown in Figure 1.12b, the heating effect of electrons is now at thetungsten electrode rather than at the workpiece. Consequently, a shallow weldis produced. Furthermore, a large-diameter, water-cooled electrodes must beused in order to prevent the electrode tip from melting. The positive ions ofthe shielding gas bombard the workpiece, as shown in Figure 1.13, knockingoff oxide ﬁlms and producing a clean weld surface. Therefore, DCEP can be14 FUSION WELDING PROCESSESDC electrodenegativeDC electrodepositiveACdeep weld,no surface cleaningshallow weld,surface cleaningintermediatepool(a) (b) (c)Figure 1.12 Three different polarities in GTAW.
used for welding thin sheets of strong oxide-forming materials such as alu-minum and magnesium, where deep penetration is not required.C. Alternating Current (AC) Reasonably good penetration and oxidecleaning action can both be obtained, as illustrated in Figure 1.12c.This is oftenused for welding aluminum alloys.1.4.3 ElectrodesTungsten electrodes with 2% cerium or thorium have better electronemissivity, current-carrying capacity, and resistance to contamination thanpure tungsten electrodes (3). As a result, arc starting is easier and the arc ismore stable. The electron emissivity refers to the ability of the electrode tipto emit electrons. A lower electron emissivity implies a higher electrode tiptemperature required to emit electrons and hence a greater risk of melting thetip.1.4.4 Shielding GasesBoth argon and helium can be used. Table 1.2 lists the properties of someshielding gases (6). As shown, the ionization potentials for argon and heliumare 15.7 and 24.5eV (electron volts), respectively. Since it is easier to ionizeargon than helium, arc initiation is easier and the voltage drop across the arcis lower with argon. Also, since argon is heavier than helium, it offers moreeffective shielding and greater resistance to cross draft than helium. WithDCEP or AC, argon also has a greater oxide cleaning action than helium.These advantages plus the lower cost of argon make it more attractive forGTAW than helium.GAS–TUNGSTEN ARC WELDING 15Cleaning action (electrode positive)knocked-off atomsoxide film on surfaceM M MOOOMWorkpiece (negative)Ar+bombarding heavy ionFigure 1.13 Surface cleaning action in GTAW with DC electrode positive.
Because of the greater voltage drop across a helium arc than an argon arc,however, higher power inputs and greater sensitivity to variations in the arclength can be obtained with helium. The former allows the welding of thickersections and the use of higher welding speeds. The latter, on the other hand,allows a better control of the arc length during automatic GTAW.1.4.5 Advantages and DisadvantagesGas–tungsten arc welding is suitable for joining thin sections because of itslimited heat inputs. The feeding rate of the ﬁller metal is somewhat indepen-dent of the welding current, thus allowing a variation in the relative amountof the fusion of the base metal and the fusion of the ﬁller metal. Therefore,the control of dilution and energy input to the weld can be achieved withoutchanging the size of the weld. It can also be used to weld butt joints of thinsheets by fusion alone, that is, without the addition of ﬁller metals or autoge-nous welding. Since the GTAW process is a very clean welding process, it canbe used to weld reactive metals, such as titanium and zirconium, aluminum,and magnesium.However, the deposition rate in GTAW is low. Excessive welding currentscan cause melting of the tungsten electrode and results in brittle tungsteninclusions in the weld metal. However, by using preheated ﬁller metals, thedeposition rate can be improved. In the hot-wire GTAW process, the wire isfed into and in contact with the weld pool so that resistance heating can beobtained by passing an electric current through the wire.1.5 PLASMA ARC WELDING1.5.1 The ProcessPlasma arc welding (PAW) is an arc welding process that melts and joins metalsby heating them with a constricted arc established between a tungsten elec-16 FUSION WELDING PROCESSESTABLE 1.2 Properties of Shielding Gases Used for WeldingMolecular Speciﬁc Gravity IonizationChemical Weight with Respect to Air Density PotentialGas Symbol (g/mol) at 1atm and 0°C (g/L) (eV)Argon Ar 39.95 1.38 1.784 15.7Carbon dioxide CO2 44.01 1.53 1.978 14.4Helium He 4.00 0.1368 0.178 24.5Hydrogen H2 2.016 0.0695 0.090 13.5Nitrogen N2 28.01 0.967 1.25 14.5Oxygen O2 32.00 1.105 1.43 13.2Source: Reprinted from Lyttle (6).
trode and the metals, as shown in Figure 1.14. It is similar to GTAW, but anoriﬁce gas as well as a shielding gas is used.As shown in Figure 1.15, the arc inPAW is constricted or collimated because of the converging action of the oriﬁcegas nozzle, and the arc expands only slightly with increasing arc length (5).Direct-current electrode negative is normally used, but a special variable-polarity PAW machine has been developed for welding aluminum, where thepresence of aluminum oxide ﬁlms prevents a keyhole from being established.1.5.2 Arc InitiationThe tungsten electrode sticks out of the shielding gas nozzle in GTAW (Figure1.11b) while it is recessed in the oriﬁce gas nozzle in PAW (Figure 1.14b). Con-sequently,arc initiation cannot be achieved by striking the electrode tip againstthe workpiece as in GTAW. The control console (Figure 1.14a) allows a pilotarc to be initiated, with the help of a high-frequency generator, between theelectrode tip and the water-cooled oriﬁce gas nozzle.The arc is then graduallyPLASMA ARC WELDING 17Shielding gasPowerSourceCablesFillerrodControlconsoleWeldingdirectionTorchOrifice gasWorkpiece(a)(b)TungstenelectrodeWeldmetalOrifice gasShielding gasnozzleShieldinggasOrificeMolten metalBase metalKeyholeArc plasmaOrifice gas nozzle(water cooled)Figure 1.14 Plasma arc welding: (a) overall process; (b) welding area enlarged andshown with keyholing.
transferred from between the electrode tip and the oriﬁce gas nozzle tobetween the electrode tip and the workpiece.1.5.3 KeyholingIn addition to the melt-in mode adopted in conventional arc welding processes(such as GTAW), the keyholing mode can also be used in PAW in certainranges of metal thickness (e.g., 2.5–6.4mm). With proper combinations of theoriﬁce gas ﬂow, the travel speed, and the welding current, keyholing is possi-ble. Keyholing is a positive indication of full penetration and it allows theuse of signiﬁcantly higher welding speeds than GTAW. For example, it hasbeen reported (7) that PAW took one-ﬁfth to one-tenth as long to completea 2.5-m-long weld in 6.4-mm-thick 410 stainless steel as GTAW. Gas–tungstenarc welding requires multiple passes and is limited in welding speed.As shownin Figure 1.16, 304 stainless steel up to 13mm (1/2 in.) thick can be welded in asingle pass (8). The wine-cup-shaped weld is common in keyholing PAW.1.5.4 Advantages and DisadvantagesPlasma arc welding has several advantages over GTAW.With a collimated arc,PAW is less sensitive to unintentional arc length variations during manualwelding and thus requires less operator skill than GTAW.The short arc lengthin GTAW can cause a welder to unintentionally touch the weld pool with theelectrode tip and contaminate the weld metal with tungsten. However, PAWdoes not have this problem since the electrode is recessed in the nozzle. Asalready mentioned, the keyhole is a positive indication of full penetration, andit allows higher welding speeds to be used in PAW.However, the PAW torch is more complicated. It requires proper electrodetip conﬁguration and positioning, selection of correct oriﬁce size for the appli-cation, and setting of both oriﬁce and shielding gas ﬂow rates. Because of the18 FUSION WELDING PROCESSESPlasma arc Gas tungsten arcFigure 1.15 Comparison between a gas–tungsten arc and a plasma arc. From WeldingHandbook (5). Courtesy of American Welding Society.
need for a control console,the equipment cost is higher in PAW than in GTAW.The equipment for variable-polarity PAW is much more expensive than thatfor GTAW.1.6 GAS–METAL ARC WELDING1.6.1 The ProcessGas–metal arc welding (GMAW) is a process that melts and joins metals byheating them with an arc established between a continuously fed ﬁller wireelectrode and the metals, as shown in Figure 1.17. Shielding of the arc and themolten weld pool is often obtained by using inert gases such as argon andhelium, and this is why GMAW is also called the metal–inert gas (MIG)welding process. Since noninert gases, particularly CO2, are also used, GMAWseems a more appropriate name. This is the most widely used arc weldingprocess for aluminum alloys. Figure 1.18 shows gas–metal arc welds of 5083aluminum, one made with Ar shielding and the other with 75% He–25% Arshielding (9). Unlike in GTAW, DCEP is used in GMAW.A stable arc, smoothmetal transfer with low spatter loss and good weld penetration can beobtained. With DCEN or AC, however, metal transfer is erratic.1.6.2 Shielding GasesArgon, helium, and their mixtures are used for nonferrous metals as well asstainless and alloy steels. The arc energy is less uniformly dispersed in an Ararc than in a He arc because of the lower thermal conductivity of Ar. Conse-quently, the Ar arc plasma has a very high energy core and an outer mantleof lesser thermal energy. This helps produce a stable, axial transfer of metalGAS–METAL ARC WELDING 19Figure 1.16 A plasma arc weld made in 13-mm-thick 304 stainless steel with keyhol-ing. From Lesnewich (8).
droplets through an Ar arc plasma.The resultant weld transverse cross sectionis often characterized by a papillary- (nipple-) type penetration pattern (10)such as that shown in Figure 1.18 (left). With pure He shielding, on the otherhand, a broad, parabolic-type penetration is often observed.With ferrous metals, however, He shielding may produce spatter and Arshielding may cause undercutting at the fusion lines. Adding O2 (about 3%)or CO2 (about 9%) to Ar reduces the problems. Carbon and low-alloy steelsare often welded with CO2 as the shielding gas, the advantages being higher20 FUSION WELDING PROCESSES(b)(a)Shielding gasnozzleWeldmetalMetaldropletShieldinggasBase metal Weld poolArcShieldinggasRegulatorFlow meterWire drive& controlWirereelWireelectrodeWorkpieceGunPowerSourceShieldinggascylinderWeldingdirectionWire electrodeContact tubeCable 1Cable 2Cable 1Figure 1.17 Gas–metal arc welding: (a) overall process; (b) welding area enlarged.Figure 1.18 Gas–metal arc welds in 6.4-mm-thick 5083 aluminum made with argon(left) and 75% He–25% Ar (right). Reprinted from Gibbs (9). Courtesy of AmericanWelding Society.
welding speed, greater penetration, and lower cost. Since CO2 shielding pro-duces a high level of spatter, a relatively low voltage is used to maintain a shortburied arc to minimize spatter; that is, the electrode tip is actually below theworkpiece surface (10).1.6.3 Modes of Metal TransferThe molten metal at the electrode tip can be transferred to the weld pool bythree basic transfer modes: globular, spray, and short-circuiting.A. Globular Transfer Discrete metal drops close to or larger than theelectrode diameter travel across the arc gap under the inﬂuence of gravity.Figure 1.19a shows globular transfer during GMAW of steel at 180A andwith Ar–2% O2 shielding (11). Globular transfer often is not smooth andproduces spatter. At relatively low welding current globular transferoccurs regardless of the type of the shielding gas. With CO2 and He, however,it occurs at all usable welding currents. As already mentioned, a shortburied arc is used in CO2-shielded GMAW of carbon and low-alloy steels tominimize spatter.GAS–METAL ARC WELDING 21Figure 1.19 Metal transfer during GMAW of steel with Ar–2% O2 shielding: (a)globular transfer at 180A and 29V shown at every 3 ¥ 10-3s; (b) spray transfer at320A and 29V shown at every 2.5 ¥ 10-4s. Reprinted from Jones et al. (11). Courtesyof American Welding Society.
B. Spray Transfer Above a critical current level, small discrete metal dropstravel across the arc gap under the inﬂuence of the electromagnetic force atmuch higher frequency and speed than in the globular mode. Figure 1.19bshows spray transfer during GMAW of steel at 320A and with Ar–2% O2shielding (11). Metal transfer is much more stable and spatter free. The criti-cal current level depends on the material and size of the electrode and thecomposition of the shielding gas. In the case of Figure 1.19, the critical currentwas found to be between 280 and 320A (11).C. Short-Circuiting Transfer The molten metal at the electrode tip is trans-ferred from the electrode to the weld pool when it touches the pool surface,that is, when short circuiting occurs. Short-circuiting transfer encompasses thelowest range of welding currents and electrode diameters. It produces a smalland fast-freezing weld pool that is desirable for welding thin sections, out-of-position welding (such as overhead-position welding), and bridging large rootopenings.1.6.4 Advantages and DisadvantagesLike GTAW, GMAW can be very clean when using an inert shielding gas.Themain advantage of GMAW over GTAW is the much higher deposition rate,which allows thicker workpieces to be welded at higher welding speeds. Thedual-torch and twin-wire processes further increase the deposition rate ofGMAW (12). The skill to maintain a very short and yet stable arc in GTAWis not required. However, GMAW guns can be bulky and difﬁcult-to-reachsmall areas or corners.1.7 FLUX-CORE ARC WELDING1.7.1 The ProcessFlux-core arc welding (FCAW) is similar to GMAW, as shown in Figure 1.20a.However, as shown in Figure 1.20b, the wire electrode is ﬂux cored rather thansolid; that is, the electrode is a metal tube with ﬂux wrapped inside. The func-tions of the ﬂux are similar to those of the electrode covering in SMAW,includ-ing protecting the molten metal from air. The use of additional shielding gasis optional.1.8 SUBMERGED ARC WELDING1.8.1 The ProcessSubmerged arc welding (SAW) is a process that melts and joins metals byheating them with an arc established between a consumable wire electrode22 FUSION WELDING PROCESSES
and the metals, with the arc being shielded by a molten slag and granular ﬂux,as shown in Figure 1.21. This process differs from the arc welding processesdiscussed so far in that the arc is submerged and thus invisible.The ﬂux is sup-plied from a hopper (Figure 1.21a), which travels with the torch. No shieldinggas is needed because the molten metal is separated from the air by the moltenslag and granular ﬂux (Figure 1.21b). Direct-current electrode positive is mostoften used. However, at very high welding currents (e.g., above 900A) AC ispreferred in order to minimize arc blow. Arc blow is caused by the electro-magnetic (Lorentz) force as a result of the interaction between the electriccurrent itself and the magnetic ﬁeld it induces.1.8.2 Advantages and DisadvantagesThe protecting and reﬁning action of the slag helps produce clean welds inSAW. Since the arc is submerged, spatter and heat losses to the surroundingair are eliminated even at high welding currents. Both alloying elements andmetal powders can be added to the granular ﬂux to control the weld metalcomposition and increase the deposition rate, respectively. Using two or moreelectrodes in tandem further increases the deposition rate. Because of its highSUBMERGED ARC WELDING 23(b)(a)Shielding gasnozzleWeldmetalBase metal Weld poolArcShieldinggasRegulatorFlow meterWire drive& controlWirereelWireelectrodeWorkpieceGunPowerSourceShieldinggascylinderWeldingdirectionWire electrodeContact tubeCable 1Cable 2Cable 1SlagMetal dropletFlux dropletShielding gas(optional)Figure 1.20 Flux-core arc welding: (a) overall process; (b) welding area enlarged.
deposition rate, workpieces much thicker than that in GTAW and GMAW canbe welded by SAW. However, the relatively large volumes of molten slag andmetal pool often limit SAW to ﬂat-position welding and circumferentialwelding (of pipes). The relatively high heat input can reduce the weld qualityand increase distortions.1.9 ELECTROSLAG WELDING1.9.1 The ProcessElectroslag welding (ESW) is a process that melts and joins metals by heatingthem with a pool of molten slag held between the metals and continuouslyfeeding a ﬁller wire electrode into it, as shown in Figure 1.22. The weld poolis covered with molten slag and moves upward as welding progresses. A pairof water-cooled copper shoes, one in the front of the workpiece and onebehind it, keeps the weld pool and the molten slag from breaking out. Similarto SAW, the molten slag in ESW protects the weld metal from air and reﬁnesit. Strictly speaking, however, ESW is not an arc welding process, because thearc exists only during the initiation period of the process, that is, when the arc24 FUSION WELDING PROCESSESWire reelWire electrodeWire drive & controlCablesFlux hopperWorkpieceGranularflux Wire electrodeArc Molten slagSolidified slagMetal pool(a)(b)WeldingdirectionWeld metalBase metalPowerSourceDropletFigure 1.21 Submerged arc welding: (a) overall process; (b) welding area enlarged.
heats up the ﬂux and melts it. The arc is then extinguished, and the resistanceheating generated by the electric current passing through the slag keeps itmolten. In order to make heating more uniform, the electrode is often oscil-lated, especially when welding thicker sections. Figure 1.23 is the transversecross section of an electroslag weld in a steel 7cm thick (13).Typical examplesof the application of ESW include the welding of ship hulls, storage tanks, andbridges.1.9.2 Advantages and DisadvantagesElectroslag welding can have extremely high deposition rates, but only onesingle pass is required no matter how thick the workpiece is. Unlike SAW orother arc welding processes, there is no angular distortion in ESW because theELECTROSLAG WELDING 25Wire electrodeConsumableguide tubeBase metalMolten slagWeld poolWeld metalCableWater-cooledcoppershoesCableWorkpieceWirereelPowerSourceWire feedmotor & controlBottomsupport(a)(b)Figure 1.22 Electroslag welding: (a) overall process; (b) welding area enlarged.
weld is symmetrical with respect to its axis. However, the heat input is veryhigh and the weld quality can be rather poor, including low toughness causedby the coarse grains in the fusion zone and the heat-affected zone. Electroslagwelding is restricted to vertical position welding because of the very largepools of the molten metal and slag.Figure 1.24 summarizes the deposition rates of the arc welding processesdiscussed so far (14). As shown, the deposition rate increases in the order of26 FUSION WELDING PROCESSESFigure 1.23 Transverse cross section of electroslag weld in 70-mm-thick steel.Reprinted from Eichhorn et al. (13). Courtesy of American Welding Society.Deposition Rate, Lb/hrWeldingProcess(100%DutyCycle)6010601270187024coldwirefine wiresprayCO2 shieldedwith iron powder added1 electrode2 electrodes4 electrodes5 electrodes3 electrodesSMAWGTAW/PAWGMAWFCAWSAWESW0 40 80 120 160 200Deposition Rate, Kg/hr8020 40 600iron powderFigure 1.24 Deposition rate in arc welding processes. Modiﬁed from Cary (14).
GTAW, SMAW, GMAW and FCAW, SAW, and ESW. The deposition rate canbe much increased by adding iron powder in SAW or using more than onewire in SAW, ESW, and GMAW (not shown).1.10 ELECTRON BEAM WELDING1.10.1 The ProcessElectron beam welding (EBW) is a process that melts and joins metals byheating them with an electron beam.As shown in Figure 1.25a, the cathode ofthe electron beam gun is a negatively charged ﬁlament (15). When heated upto its thermionic emission temperature, this ﬁlament emits electrons. Theseelectrons are accelerated by the electric ﬁeld between a negatively chargedbias electrode (located slightly below the cathode) and the anode. They passthrough the hole in the anode and are focused by an electromagnetic coil toa point at the workpiece surface. The beam currents and the acceleratingvoltages employed for typical EBW vary over the ranges of 50–1000mA and30–175kV, respectively. An electron beam of very high intensity can vaporizethe metal and form a vapor hole during welding, that is, a keyhole, as depictedin Figure 1.25b.Figure 1.26 shows that the beam diameter decreases with decreasingambient pressure (1). Electrons are scattered when they hit air molecules, andthe lower the ambient pressure, the less they are scattered. This is the mainreason for EBW in a vacuum chamber.The electron beam can be focused to diameters in the range of 0.3–0.8mmand the resulting power density can be as high as 1010W/m2(1). The very highELECTRON BEAM WELDING 27weldingdirectionweldbeadelectronbeamkeyholeweld poolcross-sectionof weld(b)motenmetalelectronbeamspecimenbiaselectrodeanodefocusingcoiltopumphighvoltagecathode(a)vacuumchamberFigure 1.25 Electron beam welding: (a) process; (b) keyhole. Modiﬁed from Arata(15).
power density makes it possible to vaporize the material and produce a deep-penetrating keyhole and hence weld. Figure 1.27 shows a single-pass electronbeam weld and a dual-pass gas–tungsten arc weld in a 13-mm-thick (0.5-in.)2219 aluminum, the former being much narrower (16). The energy requiredper unit length of the weld is much lower in the electron beam weld (1.5kJ/cm,or 3.8kJ/in.) than in the gas–tungsten arc weld (22.7kJ/cm, or 57.6kJ/in.).Electron beam welding is not intended for incompletely degassed materi-als such as rimmed steels. Under high welding speeds gas bubbles that do nothave enough time to leave deep weld pools result in weld porosity. Materialscontaining high-vapor-pressure constituents, such as Mg alloys and Pb-containing alloys, are not recommended for EBW because evaporation ofthese elements tends to foul the pumps or contaminate the vacuum system.1.10.2 Advantages and DisadvantagesWith a very high power density in EBW, full-penetration keyholing is possi-ble even in thick workpieces. Joints that require multiple-pass arc welding can28 FUSION WELDING PROCESSES750 torr 500 torr 250 torr 50 torr 5 torrFigure 1.26 Dispersion of electron beam at various ambient pressures (1). Reprintedfrom Welding Handbook (1). Courtesy of American Welding Society.13 mm(0.5 in)electronbeamweldgastungstenarc weld(a) (b)Figure 1.27 Welds in 13-mm-thick 2219 aluminum: (a) electron beam weld; (b)gas–tungsten arc weld. From Farrell (16).
be welded in a single pass at a high welding speed. Consequently, the totalheat input per unit length of the weld is much lower than that in arc welding,resulting in a very narrow heat-affected zone and little distortion. Reactiveand refractory metals can be welded in vacuum where there is no air to causecontamination. Some dissimilar metals can also be welded because the veryrapid cooling in EBW can prevent the formation of coarse, brittle intermetal-lic compounds.When welding parts varying greatly in mass and size, the abilityof the electron beam to precisely locate the weld and form a favorably shapedfusion zone helps prevent excessive melting of the smaller part.However, the equipment cost for EBW is very high. The requirement ofhigh vacuum (10-3–10-6torr) and x-ray shielding is inconvenient and time con-suming. For this reason, medium-vacuum (10-3–25torr) EBW and nonvacuum(1atm) EBW have also been developed. The ﬁne beam size requires preciseﬁt-up of the joint and alignment of the joint with the gun. As shown in Figure1.28, residual and dissimilar metal magnetism can cause beam deﬂection andresult in missed joints (17).1.11 LASER BEAM WELDING1.11.1 The ProcessLaser beam welding (LBW) is a process that melts and joins metals by heatingthem with a laser beam. The laser beam can be produced either by a solid-LASER BEAM WELDING 29Missedjoint48356 47421A387SB49Figure 1.28 Missed joints in electron beam welds in 150-mm-thick steels: (a)2.25Cr–1Mo steel with a transverse ﬂux density of 3.5G parallel to joint plane; (b) SB(C–Mn) steel and A387 (2.25Cr–1Mo) steel. Reprinted from Blakeley and Sanderson(17). Courtesy of American Welding Society.(a) (b)
state laser or a gas laser. In either case, the laser beam can be focused anddirected by optical means to achieve high power densities. In a solid-statelaser, a single crystal is doped with small concentrations of transition elementsor rare earth elements. For instance, in a YAG laser the crystal of yttrium–aluminum–garnet (YAG) is doped with neodymium. The electrons of thedopant element can be selectively excited to higher energy levels upon expo-sure to high-intensity ﬂash lamps, as shown in Figure 1.29a. Lasing occurs whenthese excited electrons return to their normal energy state, as shown in Figure1.29b.The power level of solid-state lasers has improved signiﬁcantly, and con-tinuous YAG lasers of 3 or even 5kW have been developed.In a CO2 laser, a gas mixture of CO2, N2, and He is continuously excitedby electrodes connected to the power supply and lases continuously. Higher30 FUSION WELDING PROCESSES(a)PowersourceCoolingsystemReflecting mirrorPatially reflecting mirrorFocusing lensTraveldirectionPool WeldWorkpieceCrystalHighintensityflashlamp(b)energy absorbedfrom flash lampenergy emittedas heatenergyemitted aslight (photon)nucleusgroundintermediateexcitedinnerelectronsouterelectronenergylevelsnormalelectronorbitsFigure 1.29 Laser beam welding with solid-state laser: (a) process; (b) energy absorp-tion and emission during laser action. Modiﬁed from Welding Handbook (1).
power can be achieved by a CO2 laser than a solid-state laser, for instance,15kW. Figure 1.30a shows LBW in the keyholing mode. Figure 1.30b shows aweld in a 13-mm-thick A633 steel made with a 15-kW CO2 laser at 20mm/s(18).Besides solid-state and gas lasers, semiconductor-based diode lasers havealso been developed. Diode lasers of 2.5kW power and 1mm focus diameterhave been demonstrated (19).While keyholing is not yet possible, conduction-mode (surface melting) welding has produced full-penetration welds with adepth–width ratio of 3:1 or better in 3-mm-thick sheets.1.11.2 ReﬂectivityThe very high reﬂectivity of a laser beam by the metal surface is a well-knownproblem in LBW. As much as about 95% of the CO2 beam power can bereﬂected by a polished metal surface. Reﬂectivity is slightly lower with a YAGlaser beam. Surface modiﬁcations such as roughening, oxidizing, and coatingcan reduce reﬂectivity signiﬁcantly (20).Once keyholing is established,absorp-tion is high because the beam is trapped inside the hole by internal reﬂection.1.11.3 Shielding GasA plasma (an ionic gas) is produced during LBW, especially at high powerlevels, due to ionization by the laser beam. The plasma can absorb and scatterthe laser beam and reduce the depth of penetration signiﬁcantly. It is there-fore necessary to remove or suppress the plasma (21). The shielding gas forprotecting the molten metal can be directed sideways to blow and deﬂect theplasma away from the beam path. Helium is often preferred to argon as theshielding gas for high-power LBW because of greater penetration depth (22).LASER BEAM WELDING 31weldingdirectionweldbeadlaserbeamkeyholeweld poolcross-sectionof weld(a) (b)moltenmetal2 mmFigure 1.30 Laser beam welding with CO2 laser: (a) process; (b) weld in 13-mm-thickA633 steel. (b) Courtesy of E.A. Metzbower.
Since the ionization energy of helium (24.5eV) is higher than that of argon(15.7eV), helium is less likely to be ionized and become part of the plasmathan argon. However, helium is lighter than air and is thus less effective in dis-placing air from the beam path. Helium–10% Ar shielding has been foundto improve penetration over pure He at high-speed welding where a lightshielding gas may not have enough time to displace air from the beam path(23).1.11.4 Lasers in Arc WeldingAs shown in Figure 1.31, laser-assisted gas metal arc welding (LAGMAW) hasdemonstrated signiﬁcantly greater penetration than conventional GMAW(24). In addition to direct heating, the laser beam acts to focus the arc byheating its path through the arc. This increases ionization and hence the con-ductivity of the arc along the beam path and helps focus the arc energy alongthe path. It has been suggested that combining the arc power with a 5-kW CO2laser, LAGMAW has the potential to achieve weld penetration in mild steelequivalent to that of a 20–25-kW laser (24). Albright et al. (25) have shownthat a lower power CO (not CO2) laser of 7W and 1mm diameter can initi-ate, guide, and focus an Ar–1% CO gas–tungsten arc.1.11.5 Advantages and DisadvantagesLike EBW, LBW can produce deep and narrow welds at high welding speeds,with a narrow heat-affected zone and little distortion of the workpiece. It can32 FUSION WELDING PROCESSESLAGMAWGMAW300 400 500 600 700024681012Welding current (A)Penetration(mm)Figure 1.31 Weld penetration in GMAW and laser-assisted GMAW using CO2 laserat 5.7kW. Reprinted from Hyatt et al. (24). Courtesy of American Welding Society.
be used for welding dissimilar metals or parts varying greatly in mass and size.Unlike EBW, however, vacuum and x-ray shielding are not required in LBW.However, the very high reﬂectivity of a laser beam by the metal surface is amajor drawback, as already mentioned. Like EBW, the equipment cost is veryhigh, and precise joint ﬁt-up and alignment are required.REFERENCES1. Welding Handbook, Vol. 3, 7th ed., American Welding Society, Miami, FL, 1980,pp. 170–238.2. Mendez, P. F., and Eagar, T. W., Advanced Materials and Processes, 159: 39,2001.3. Welding Handbook, Vol. 1, 7th ed., American Welding Society, Miami, FL, 1976,pp. 2–32.4. Welding Workbook, Data Sheet 212a, Weld. J., 77: 65, 1998.5. Welding Handbook, Vol. 2, 7th ed., American Welding Society, Miami, FL, 1978,pp. 78–112, 296–330.6. Lyttle, K. A., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH,1993, p. 64.7. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979, pp. 2–1 to3–40.8. Lesnewich, A., in Weldability of Steels, 3rd ed., Eds. R. D. Stout and W. D. Doty,Welding Research Council, New York, 1978, p. 5.9. Gibbs, F. E., Weld. J., 59: 23, 1980.10. Fact Sheet—Choosing Shielding for GMA Welding, Weld. J., 79: 18, 2000.11. Jones, L. A., Eagar, T. W., and Lang, J. H., Weld. J., 77: 135s, 1998.12. Blackman, S. A., and Dorling, D. V., Weld. J., 79: 39, 2000.13. Eichhorn, F., Remmel, J., and Wubbels, B., Weld. J., 63: 37, 1984.14. Cary, H. B., Modern Welding Technology, Prentice-Hall, Englewood Cliffs, NJ,1979.15. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Appli-cation to Heat Processing, Okada Memorial Japan Society, 1985.16. Farrell, W. J., The Use of Electron Beam to Fabricate Structural Members, CreativeManufacturing Seminars, ASTME Paper SP 63-208, 1962–1963.17. Blakeley, P. J., and Sanderson, A., Weld. J., 63: 42, 1984.18. Metzbower, E. A., private communication, Naval Research Laboratory,Washington, DC.19. Bliedtner, J., Heyse, Th., Jahn, D., Michel, G., Muller, H., and Wolff, D., Weld. J., 80:47, 2001.20. Xie, J., and Kar, A., Weld. J., 78: 343s, 1999.21. Mazumder, J., in ASM Handbook, Vol. 6, ASM International, Materials Park, OH,1993, p. 874.22. Rockstroh, T., and Mazumder, J., J. Appl. Phys., 61: 917, 1987.REFERENCES 33
23. Seaman, F., Role of Shielding Gas in Laser Welding, Technical Paper MR77-982,Society of Manufacturing Engineers, Dearborn, MI, 1977.24. Hyatt, C. V., Magee, K. H., Porter, J. F., Merchant, V. E., and Matthews, J. R., Weld.J., 80: 163s, 2001.25. Albright, C. E., Eastman, J., and Lempert, W., Weld. J., 80: 55, 2001.26. Ushio, M., Matsuda, F., and Sadek, A. A., in “ International Trends in WeldingScience and Technology, Eds. S. A. David and J. M. Vitek, ASM International,Materials Park, OH, March 1993, p. 408.FURTHER READING1. Arata, Y., Development of Ultra High Energy Density Heat Source and Its Applica-tion to Heat Processing, Okada Memorial Society for the Promotion of Welding,Japan, 1985.2. Schwartz, M. M., Metals Joining Manual, McGraw-Hill, New York, 1979.3. Welding Handbook, Vols. 1–3, 7th ed., American Welding Society, Miami, FL,1980.4. Duley, W. W., Laser Welding, Wiley, New York, 1999.5. ASM Handbook, Vol. 6, ASM International, Materials Park, OH, 1993.PROBLEMS1.1 It has been suggested that compared to SMAW, the cooling rate ishigher in GMAW and it is, therefore, more likely for heat-affected zonecracking to occur in hardenable steels. What is the main reason for thecooling rate to be higher in GMAW than SMAW?1.2 The diameter of the electrodes to be used in SMAW depends on factorssuch as the workpiece thickness, the welding position, and the jointdesign. Large electrodes, with their corresponding high currents, tend toproduce large weld pools. When welding in the overhead or verticalposition, do you prefer using larger or smaller electrodes?1.3 In arc welding, the magnetic ﬁeld induced by the welding currentpassing through the electrode and the workpiece can interact with thearc and cause “arc blow.” Severe arc blow can cause excessive weldspatter and incomplete fusion. When arc blow is a problem in SMAW,do you expect to minimize it by using DC or AC for welding?1.4 In the hot-wire GTAW process, shown in Figure P1.4, the tip of the ﬁllermetal wire is dipped in the weld pool and the wire itself is resistanceheated by means of a second power source between the contact tube ofthe wire and the workpiece. In the case of steels, the deposition rate can34 FUSION WELDING PROCESSES
be more than doubled this way. Do you prefer using an AC or a DCpower source for heating the wire? Do you expect to apply this processto aluminum and copper alloys?1.5 In GTAW the welding cable is connected to the tungsten electrodethrough a water-cooled copper contact tube, as shown in Figure 1.11.Why is the tube positioned near the lower end of the electrode insteadof the top?1.6 Measurements of the axial temperature distribution along the GTAWelectrode have shown that the temperature drops sharply from theelectrode tip toward the contact tube. Why? For instance, with a2.4-mm-diameter W–ThO2 electrode at 150A, the temperature dropsfrom about 3600K at the tip to about 2000K at 5mm above the tip.Under the same condition but with a W–CeO2 electrode, the tempera-ture drops from about 2700K at the tip to about 1800K at 5mm abovethe tip (26).Which electrode can carry more current before melting andwhy?1.7 Experimental results show that in EBW the penetration depth of theweld decreases as the welding speed increases. Explain why. Under thesame power and welding speed, do you expect a much greater penetra-tion depth in aluminum or steel and why?1.8 How does the working distance in EBW affect the depth–width ratio ofthe resultant weld?1.9 Consider EBW in the presence of a gas environment. Under the samepower and welding speed, rank and explain the weld penetration for Ar,He, and air. The speciﬁc gravities of Ar, He, and air with respect to airare 1.38, 0.137, and 1, respectively, at 1atm, 0°C.PROBLEMS 35Shieldinggas nozzleWeldmetalShieldinggasBase metal Weld poolArcTungsten electrodeContact tubeCable 1Wire feederFiller wire2ndpowersourceCable 3Cable 4Contact tubeFigure P1.4
1.10 Which arc welding process could have been used for joining the edgeweld of thin-gauge steel shown in Figure P1.10 and why?1.11 Two 15-cm-thick steel plates were joined together in a single pass, asshown in Figure P1.11.Which welding process could have been used andwhy?36 FUSION WELDING PROCESSESweld1 mm1 mmtransversecross-sectionFigure P1.1015 cm15 cmweld transversecross-sectionsteelsteelFigure P1.11
2 Heat Flow in WeldingHeat ﬂow during welding, as will be shown throughout Parts II–IV of thisbook, can strongly affect phase transformations during welding and thus theresultant microstructure and properties of the weld. It is also responsible forweld residual stresses and distortion, as will be discussed in Chapter 5.2.1 HEAT SOURCE2.1.1 Heat Source EfﬁciencyA. Deﬁnition The heat source efﬁciency h is deﬁned as(2.1)where Q is the rate of heat transfer from the heat source to the workpiece,Qnominal the nominal power of the heat source, and tweld the welding time. Aportion of the power provided by the heat source is transferred to the work-piece and the remaining portion is lost to the surroundings. Consequently,h < 1. If the heat source efﬁciency h is known, the heat transfer rate to theworkpiece, Q, can be easily determined from Equation (2.1).In arc welding with a constant voltage E and a constant current I, the arcefﬁciency can be expressed as(2.2)Equation (2.2) can also be applied to electron beam welding, where h is theheat source efﬁciency. In laser beam welding, Qnominal in Equation (2.1) is thepower of the laser beam, for instance, 2500W.It should be noted that in the welding community the term heat input oftenrefers to Qnominal, or EI in the case of arc welding, and the term heat input perunit length of weld often refers to the ratio Qnominal/V, or EI/V, where V is thewelding speed.B. Measurements The heat source efﬁciency can be measured with acalorimeter. The heat transferred from the heat source to the workpiece is inh = =QtEItQEIweldweldh = =QtQ tQQweldnominal weld nominal37Welding Metallurgy, Second Edition. Sindo KouCopyright 2003 John Wiley & Sons, Inc.ISBN: 0-471-43491-4
turn transferred from the workpiece to the calorimeter, which can be deter-mined as described below.Kou et al. (1, 2) used simple tubular calorimeters to determine the arcefﬁciency in GTAW of aluminum, as shown in Figure 2.1a. The calorimetercan be a round cross section if the workpiece is a pipe or a rectangularcross section if the workpiece is a sheet. The temperature rise in the cool-ing water (Tout - Tin) can be measured using thermocouples or thermistors.Heat transfer from the workpiece to the calorimeter is as follows (1–3):(2.3)where W is the mass ﬂow rate of water, C the speciﬁc heat of water, Tout theoutlet water temperature, Tin the inlet water temperature, and t time.The inte-gral corresponds to the shaded area in Figure 2.1b.The arc efﬁciency h can bedetermined from Equations (2.2) and (2.3).Giedt et al. (4) used the Seebeck envelop calorimeter shown in Figure 2.2ato measure the arc efﬁciency in GTAW. The name Seebeck came fromthe Seebeck thermoelectric effect of a thermocouple, namely, a voltage isproduced between two thermocouple junctions of different temperatures.The torch can be quickly withdrawn after welding, and the calorimeter lidcan be closed to minimize heat losses to the surrounding air. As shown inFigure 2.2b, heat transfer from the workpiece to the calorimeter can bedetermined by measuring the temperature difference DT and hence gradientQt WC T T dt WC T T dtweld out in out in= -( ) ª -( )• •Ú Ú0 038 HEAT FLOW IN WELDINGGTAWtorchPipeWater outThermocoupleThermocoupleWater inInsulationArcTime, secondsTemperature,oCTemperature,oF(a)(b)100 1201201008020304050ToutTinShaded area∞= ∫ [ ]dtout- in0 T TFigure 2.1 Measurement of arc efﬁciency in GTAW: (a) calorimeter; (b) rise in coolingwater temperature as a function of time. Modiﬁed from Kou et al. (1, 2).
across a “gradient layer” of material of known thermal conductivity k andthickness L:(2.4)Qt A kTLdtweld =•ÚD0HEAT SOURCE 39TLCooling water flowGradient layerThermocouplejunctions for sensingtemperaturedifferenceDirection ofheat flowTemperatureDistanceTemperatureprofile∆Figure 2.2 Measurement of arc efﬁciency in GTAW: (a) calorimeter; (b) layer of tem-perature gradient. Reprinted from Giedt et al. (4). Courtesy of American WeldingSociety.(a)(b)
where A is the area for heat ﬂow and DT/L the temperature gradient. The arcefﬁciency h can be determined from Equations (2.4) and (2.2). This type ofcalorimeter was later used to determine the arc efﬁciencies in PAW, GMAW,and SAW (5–8).Figure 2.3 shows the results of arc efﬁciency measurements in GTAW andPAW (2, 5, 7, 9), and Figure 2.4 shows similar results in GMAW and SAW (7,10).These results were obtained using the two types of calorimeters describedabove except for the results of Lu and Kou for GMAW (10, 11), which aredescribed in what follows.In GMAW the arc, metal droplets, and cathode heating all contribute to theefﬁciency of the heat source. It has been observed in GMAW of aluminumand steel with Ar shielding that current ﬂow or electron emission occurs not40 HEAT FLOW IN WELDING1.00.80.60.40.20.0ArcEfficiency10 20 300Travel Speed, mm/sPAW:GTAW:Fuerschbach et al. (1991)Dupont et al. (1995)Kou and Lu (1985)Fuerschbach et al. (1991)Dupont et al. (1995)GTAWEvans et al. (1998)PAWFigure 2.3 Arc efﬁciencies in GTAW and PAW.175 275 375 425225 325ArcEfficiency1.00.80.60.40.212575GMAW:SAW:Lu and Kou (1989)DuPont et al. (1995)SAWGMAWCurrent, ALu and Kou (1989)DuPont et al. (1995)Figure 2.4 Arc efﬁciencies in GMAW and SAW.
uniformly over the workpiece surface but over localized areas on the work-piece surface called cathode spots (12, 13). The localized heating, calledcathode heating, causes the surface oxide to dissociate and leaves a clean metalsurface (12). Cathode heating is attributed to ﬁeld-type emission of electrons.Unlike thermionic emission at the tungsten electrode in DC electrode-negative GTAW, ﬁeld emission electrons do not cool the cathode (6).Lu and Kou (10, 11) used a combination of three calorimeters to estimatethe amounts of heat transfer from the arc, ﬁller metal droplets, and cathodeheating to the workpiece in GMAW of aluminum. Figure 2.5a shows the mea-surement of heat transfer from droplets (11). The arc is established betweena GMAW torch and a GTA torch and the droplets collect in the calorimeterbelow. From the water temperature rise and the masses and speciﬁc heats ofthe water and the copper basin, the heat transfer from droplets can be deter-HEAT SOURCE 41Filler wireGTAW torchGMAWtorchDropletsWaterRadiation baffleThermistorInsulationCubasinFiller wireGMAW torchWeldO-ringWater inWater outDTDTWorkpieceInsulationDT: differentialthermistor(b)Filler wireGMAW torchWeldO-ringWater inWater outDTDTWorkpieceInsulation(c)GTAWtorch(a)Figure 2.5 Calorimeter for measuring heat inputs in GMAW: (a) metal droplets; (b)total heat input; (c) combined heat inputs from arc and metal droplets. Reprinted fromLu and Kou (10, 11). Courtesy of American Welding Society.
mined. Figure 2.5b shows the measurement of the total heat transfer to theworkpiece. Figure 2.5c shows the measurement of the combined heat transferfrom the arc and the droplets, with cathode heating shifted to the tungstenelectrode of a nearby GTAW torch (10). The results are shown in Figure 2.6a.By subtracting the combined heat transfer from the arc and droplets from thetotal heat transfer to the workpiece, heat transfer from cathode heating wasdetermined. Figure 2.6b shows the breakdown of the total heat transfer to theworkpiece into those from the arc, droplets, and cathode heating. Within therange of the power studied, the overall efﬁciency was about 80%, with about45% from the arc, 25% from droplets, and 10% from cathode heating.The heat source efﬁciency can be very low in LBW because of the highreﬂectivity of metal surfaces to a laser beam, for instance, 98% for CO2 laseron polished aluminum. The reﬂectivity can be found by determining the ratioof the reﬂected beam power to the incident beam power. Xie and Kar (14)show that roughening the surface with sandpapers and oxidizing the surfaceby brief exposure to high temperatures can reduce the reﬂectivity signiﬁcantly.C. Heat Source Efﬁciencies in Various Welding Processes Figure 2.7 sum-marizes the heat source efﬁciencies measured in several welding processes. Afew comments are made as follows:LBW: The heat source efﬁciency is very low because of the high reﬂectiv-ity of metal surfaces but can be signiﬁcantly improved by surface modi-ﬁcations, such as roughening, oxidizing, or coating.PAW: The heat source efﬁciency is much higher than LBW because reﬂec-tivity is not a problem.GTAW: Unlike in PAW there are no heat losses from the arc plasma to thewater-cooled constricting torch nozzle. With DCEN, the imparting elec-trons are a major source of heat transfer to the workpiece. They releasethe work function as heat and their kinetic energy is also converted into42 HEAT FLOW IN WELDINGGMAW1.6 mm (1/16 in)4043 filler metalTotalArc +dropletsDropletsCurrent x voltage, kW0 2 4 6 80Powerinputs,kW246 GMAW1.6 mm (1/16 in)4043 filler metalTotalArcDropletsCathodeCurrent x voltage, kWPowerinputs,%0 2 4 6 8020406080(a) (b)Figure 2.6 Power inputs during GMAW of aluminum: (a) measured results; (b) break-down of total power input. Reprinted from Lu and Kou (10). Courtesy of AmericanWelding Society.
heat at the workpiece. In AC GTAW, however, electrons bombard theworkpiece only during the electrode-negative half cycle, and the arc efﬁ-ciency is thus lower. In GTAW with DCEP, the arc efﬁciency is evenlower because the electrons bombard the electrode rather than theworkpiece.GMAW, SMAW: Unlike in GTAW, heat transfer to the electrode can betransferred back to the workpiece through metal droplets, thus improv-ing the arc efﬁciency.SAW: Unlike in GMAW or SMAW,the arc is covered with a thermally insu-lating blanket of molten slag and granular ﬂux, thus reducing heat lossesto the surroundings and improving the arc efﬁciency.EBW: The keyhole in EBW acts like a “black body” trapping the energyfrom the electron beam. As a result, the efﬁciency of the electron beamis very high.2.1.2 Melting EfﬁciencyThe ability of the heat source to melt the base metal (as well as the ﬁller metal)is of practical interest to the welder. Figure 2.8 shows the cross-sectional areaHEAT SOURCE 43EBWSAWGMAWGTAWdcenPAWLBWHeatSourceEfficiency1.00.80.60.40.20SMAWsurfacemodificationsFigure 2.7 Heat source efﬁciencies in several welding processes.AfillerAbaseFigure 2.8 Transverse cross section of weld showing areas representing contributionsfrom base metal and ﬁller metal.
representing the portion of the weld metal contributed by the base metal, Abase,and that contributed by the ﬁller metal, Aﬁller. One way to deﬁne the meltingefﬁciency of the welding arc, hm, is as follows:(2.5)where V is the welding speed, Hbase the energy required to raise a unit volumeof base metal to the melting point and melt it, and Hﬁller the energy required toraise a unit volume of ﬁller metal to the melting point and melt it.The quantityinside the parentheses represents the volume of material melted while thedenominator represents the heat transfer from the heat source to the workpiece.Figures 2.9a and b show the transverse cross section of two steel welds dif-fering in the melting efﬁciency (7). Here, EI = 3825W and V = 10mm/s for theshallower weld of lower melting efﬁciency (Figure 2.9a) and EI = 10170W andV = 26mm/s for the deeper weld of higher melting efﬁciency (Figure 2.9b).Note that the ratio EI/V is equivalent in each case.hhmbase weld base ﬁller weld ﬁllerweld=( ) + ( )A Vt H A Vt HEIt44 HEAT FLOW IN WELDINGPAWGTAWGMAWSAWMeltingefficiency0 1000 2000 3000 4000 50000.00.10.20.126.96.36.199.7(c) −η = η αν 1750.50expm EIV/(H )ηEIV/(Hαν)Figure 2.9 Melting efﬁciency: (a) lower at lower heat input and welding speed; (b)higher at higher heat input and welding speed; (c) variation with dimensionless para-meter hEIV/Ha. Reprinted from DuPont and Marder (7). Courtesy of AmericanWelding Society.
Fuerschbach and Knorovsky (5) proposed the following empirical equationfor the melting efﬁciency:(2.6)where A and B are constants, H = Hbase + Hﬁller, a is the thermal diffusivity, and is the kinematic viscosity of the weld pool.The results of DuPont and Marder(7) shown in Figure 2.9c conﬁrms the validity of Equation (2.6). As thedimensionless parameter hEIV/Ha increases, the melting efﬁciency increasesrapidly ﬁrst and then levels off. If the arc efﬁciency h is known, hEIV/Ha isalso known and the melting efﬁciency can be predicted from Figure 2.9. Withthe help of the following equation for determining Aﬁller, Abase can then becalculated from Equation (2.5):AﬁllerVtweld = pR2ﬁllerVﬁllertweld (2.7)or(2.8)In the above equations Rﬁller and Vﬁller are the radius and feeding speed of theﬁller metal, respectively. The left-hand side of Equation (2.7) is the volume ofthe weld metal contributed by the ﬁller metal while the right-hand side is thevolume of ﬁller metal used during welding.It should be noted that the melting efﬁciency cannot be increased indeﬁ-nitely by increasing the welding speed without increasing the power input. Todo so, the power input must be increased along with the welding speed. Itshould also be noted that in the presence of a surface-active agent suchas sulfur in steel, the weld pool can become much deeper even thoughthe welding parameters and physical properties in Equation (2.6) remainunchanged (Chapter 4).2.1.3 Power Density Distribution of Heat SourceA. Effect of Electrode Tip Angle In GTAW with DCEN, the shape of theelectrode tip affects both the shape and power density distribution of thearc. As the electrode tip becomes blunter, the diameter of the arc decreasesand the power density distribution increases, as illustrated in Figure 2.10.Glickstein (15) showed, in Figure 2.11, that the arc becomes more constrictedas the conical tip angle of the tungsten electrode increases.Savage et al. (16) observed that, under the same welding current, speed, andarc gap, the weld depth–width ratio increases with increasing vertex angle ofAR VVﬁllerﬁller2ﬁller=phh am =-ÊËˆ¯ABEIV HexpnHEAT SOURCE 45
46 HEAT FLOW IN WELDINGTungstenelectrodeArcPowerdensityRadialdistancePowerdensityRadialdistance(a)(b)(c)(d)Figure 2.10 Effect of electrode tip angle on shape and power density distribution ofgas–tungsten arc.Figure 2.11 Effect of electrode tip angle on shape of gas–tungsten arc. Reprinted fromGlickstein (15).
the conical tip of the tungsten electrode. Key (17) reported a similar effect ofthe tip angle, at least with Ar shielding, as shown in Figure 2.12.B. Measurements Several investigators have measured the power densitydistribution (and current density distribution) in the gas tungsten arc by usingthe split-anode method (2, 18–20). Figure 2.13 shows the results of Tsai (20)and Lu and Kou (3).For simplicity,the Gaussian-type distribution is often usedas an approximation (21–23).2.2 ANALYSIS OF HEAT FLOW IN WELDINGFigure 2.14 is a schematic showing the welding of a stationary workpiece (24).The origin of the coordinate system moves with the heat source at a constantspeed V in the negative-x direction. Except for the initial and ﬁnal transientsANALYSIS OF HEAT FLOW IN WELDING 4730o(0.125)60o(0.125)90o(0.500)180o(0)Electrode tip angle(truncation, mm)Figure 2.12 Effect of electrode tip geometry on shape of gas–tungsten arc welds instainless steel (pure Ar, 150A, 2.0s, spot-on-plate). Reprinted from Key (17). Courtesyof American Welding Society.-0.1r20 2 4 6 80204060q(r) = 30ePowerDensity,W/mm2Radius, mmLu and Kou (1988)Tsai (1983)electrode (+)100 A,14.2 V4.7 mm arc100% Ar3.2 mm electrode75 tip angleq(r) = 32e-0.1r2oFigure 2.13 Measured power density distributions. Reprinted from Lu and Kou (3).Courtesy of American Welding Society.
of welding, heat ﬂow in a workpiece of sufﬁcient length is steady, or quasi-stationary, with respect to the moving heat source. In other words, for anobserver moving with the heat source, the temperature distribution and thepool geometry do not change with time.This steady-state assumption was ﬁrstused by Rosenthal (25) to simplify the mathematical treatment of heat ﬂowduring welding.2.2.1 Rosenthal’s EquationsRosenthal (25) used the following simplifying assumptions to derive analyti-cal equations for heat ﬂow during welding:1. steady-state heat ﬂow,2. point heat source,3. negligible heat of fusion,4. constant thermal properties,5. no heat losses from the workpiece surface, and6. no convection in the weld pool.A. Rosenthal’s Two-Dimensional Equation Figure 2.15 is a schematicshowing the welding of thin sheets. Because of the small thickness of the work-piece, temperature variations in the thickness direction are assumed negligi-ble and heat ﬂow is assumed two dimensional. Rosenthal (25) derived thefollowing equation for two-dimensional heat ﬂow during the welding of thinsheets of inﬁnite width:48 HEAT FLOW IN WELDINGFigure 2.14 Coordinate system (x, y, z) moving with heat source. From Kou and Le(24).
(2.9)where T = temperatureT0 = workpiece temperature before weldingk = workpiece thermal conductivityg = workpiece thicknessQ = heat transferred from heat source to workpieceV = travel speeda = workpiece thermal diffusivity, namely, k/rC, where r and C aredensity and speciﬁc heat of the workpiece, respectivelyK0 = modiﬁed Bessel function of second kind and zero order, as shownin Figure 2.16 (26)r = radial distance from origin, namely, (x2+ y2)1/2Equation (2.9) can be used to calculate the temperature T(x, y) at any loca-tion in the workpiece (x, y) with respect to the moving heat source, forinstance, at x = -1cm and y = 4cm shown in Figure 2.15. The temperatures atother locations along y = 4cm can also be calculated, and the temperature dis-tribution along y = 4cm can thus be determined. Table 2.1 lists the thermalproperties for several materials (27).B. Rosenthal’s Three-Dimensional Equation The analytical solutionderived by Rosenthal for three-dimensional heat ﬂow in a semi-inﬁnite work-piece during welding, Figure 2.17, is as follows (25):(2.10)220paT T kRQV R x-( )=- -( )ÈÎÍ˘˚˙exp22 200pa aT T kgQVxKVr-( )=ÊËˆ¯ÊËˆ¯expANALYSIS OF HEAT FLOW IN WELDING 49thickness, gthin sheets attemperature T0before weldingheat source, Qweld poolfusion zoneT(x,y) shown at x = -1 cm and y = 4 cmy = 4 cmT(x,y)T2o1 2 3 4 50-3 -1-2yxweldingspeed, VFigure 2.15 Two-dimensional heat ﬂow during welding of thin workpiece.
where R is the radial distance from the origin, namely, (x2+ y2+ z2)1/2. For agiven material and a given welding condition, an isotherm T on a plane at agiven x has a radius of R. In other words, Equation (2.10) implies that on thetransverse cross section of the weld all isotherms, including the fusion bound-ary and the outer boundary of the heat-affected zone, are semicircular inshape. Equation (2.10) can be used to calculate the steady-state temperatureT(x, y, z), with respect to the moving heat source, at any location in the work-piece (x, y, z), for instance, at x = 1cm, y = 4cm, and z = 0cm, as shown inFigure 2.17. The temperatures at other locations along y = 4cm can also be50 HEAT FLOW IN WELDING2.82.42.01.188.8.131.520 1 2 3 4Modified Bessel functionof second kindzero orderK0[Vr/(2)]Vr/(2 )ααFigure 2.16 Modiﬁed Bessel function of second kind and zero order (26).TABLE 2.1 Thermal Properties for Several MaterialsVolumeThermal Thermal Thermal MeltingDiffusivity, Capacity, Conductivity, PointMaterial a (m2/s) rCs (J/m3K) k (J/msK) (K)Aluminum 8.5 ¥ 10-52.7 ¥ 106229.0 933Carbon steel 9.1 ¥ 10-64.5 ¥ 10641.0 18009% Ni steel 1.1 ¥ 10-53.2 ¥ 10635.2 1673Austenitic 5.3 ¥ 10-64.7 ¥ 10624.9 1773stainless steelInconel 600 4.7 ¥ 10-63.9 ¥ 10618.3 1673Ti alloy 9.0 ¥ 10-63.0 ¥ 10627.0 1923Copper 9.6 ¥ 10-54.0 ¥ 106384.0 1336Monel 400 8.0 ¥ 10-64.4 ¥ 10635.2 1573Source: Gray et al. (27).
calculated, and the temperature distribution along y = 4cm can thus bedetermined.C. Thermal Cycles and Temperature Distributions Equations (2.9) and(2.10) can be used to calculate the temperature distribution in the workpieceduring welding. The temperature distribution in the welding direction, forinstance, the T–x curves in Figures 2.15 and 2.17, are of particular interest.They can be readily converted into temperature–time plots, namely, thethermal cycles, by converting distance x into time t through t = (x - 0)/V.Figures 2.18 and 2.19 show calculated thermal cycles and temperature distri-butions at the top surface (z = 0) of a thick 1018 steel at two different sets ofheat input and welding speed. The inﬁnite peak temperature at the origin ofthe coordinate system is the result of the singularity problem in Rosenthal’ssolutions caused by the point heat source assumption.It should be mentioned, however, that Rosenthal’s analytical solutions,though based on many simplifying assumptions, are easy to use and have beengreatly appreciated by the welding industry.2.2.2 Adams’ EquationsAdams (28) derived the following equations for calculating the peak temper-ature Tp at the workpiece surface (z = 0) at a distance Y away from the fusionline (measured along the normal direction):(2.11)for two-dimensional heat ﬂow and1 4 13 10 0T TVYg CQ T Tp -= +-. rmANALYSIS OF HEAT FLOW IN WELDING 51semi-infinite platesat temperature T0before weldingheat source, Qweld poolfusion zoneweldingspeed, VT(x,y,z)y = 4 cmTo1420z-2T(x,y,z) shown at x = 1 cm, y = 4cm and z = 0 cmyxFigure 2.17 Three-dimensional heat ﬂow during welding of semi-inﬁnite workpiece.
(2.12)for three-dimensional heat ﬂow.Several other analytical solutions have also been derived for two-dimensional (29–34) and three-dimensional (31, 35–37) welding heat ﬂow.Because of the many simplifying assumptions used, analytical solutions havehad limited success.2.2.3 Computer SimulationMany computer models have been developed to study two-dimensional heatﬂow (e.g., refs. 38–43) and three-dimensional heat ﬂow (e.g., refs. 44–55) duringwelding. Most assumptions of Rosenthal’s analytical solutions are no longerrequired. Figure 2.20 shows the calculated results of Kou and Le (24) for theGTAW of 3.2-mm-thick sheets of 6061 aluminum alloy. The agreement withobserved fusion boundaries and thermal cycles appears good.1 5 44221020T TkQVVYT Tp -= +ÊËˆ¯ÈÎÍ˘˚˙ +-. p aa m52 HEAT FLOW IN WELDINGFigure 2.18 Calculated results from Rosenthal’s three-dimensional heat ﬂow equa-tion: (a) thermal cycles; (b) isotherms. Welding speed: 2.4mm/s; heat input: 3200W;material: 1018 steel.
2.3 EFFECT OF WELDING PARAMETERS2.3.1 Pool ShapeAs the heat input Q and welding speed V both increase, the weld pool becomesmore elongated, shifting from elliptical to teardrop shaped. Figure 2.21 showsthe weld pools traced from photos taken during autogenous GTAW of 304stainless steel sheets 1.6mm thick (56). Since the pools were photographedfrom the side at an inclined angle (rather than vertically), the scale bar appliesonly to lengths in the welding direction. In each pool the cross indicates theposition of the electrode tip relative to the pool.The higher the welding speed,the greater the length–width ratio becomes and the more the geometric centerof the pool lags behind the electrode tip.Kou and Le (57) quenched the weld pool during autogenous GTAW of1.6-mm 309 stainless steel sheets and observed the sharp pool end shown in Figure2.22. The welding current was 85A, voltage 10V, and speed 4.2mm/s [10in./min(ipm)].The sharp end characteristic of a teardrop-shaped weld pool is evident.The effect of the welding parameters on the pool shape is more signiﬁcantin stainless steel sheets than in aluminum sheets.The much lower thermal con-EFFECT OF WELDING PARAMETERS 53Figure 2.19 Calculated results similar to those in Figure 2.18 but with welding speedof 6.2mm/s and heat input of 5000W.
54 HEAT FLOW IN WELDINGFigure 2.20 Computer simulation of GTAW of 3.2-mm-thick 6061 aluminum, 110A,10V, and 4.23mm/s: (a) fusion boundaries and isotherms; (b) thermal cycles. From Kouand Le (24).2mm 35A, 7.4V0.42 mm/s70A, 8.4V2.5 mm/s100A, 9.0V4.2 mm/s304 stainless steel sheetsFigure 2.21 Weld pool shapes in GTAW of 304 stainless steel sheets. Courtesy ofSmolik (56).
ductivity of stainless steels makes it more difﬁcult for the weld pool to dissi-pate heat and solidify.2.3.2 Cooling Rate and Temperature GradientThe ratio EI/V represents the amount of heat input per unit length of weld.Lee et al. (58) measured the cooling rate in GTAW of 2024 aluminum by stick-ing a thermocouple into the weld pool. Figure 2.23 shows that increasing EI/VEFFECT OF WELDING PARAMETERS 55Figure 2.22 Sharp pool end in GTAW of 309 stainless steel preserved by ice quench-ing during welding. From Kou and Le (57).800(a)(b)(e)(d)(c)(f)(a) V:10 cm/min; EI/V:15.4 kJ/cm(b) V:15 cm/min; EI/V:9.79 kJ/cm(c) V:20 cm/min; EI/V:7.34 kJ/cm(d) V:30 cm/min; EI/V:4.76 kJ/cm(e) V:40 cm/min; EI/V:3.57 kJ/cm(f) V:60 cm/min; EI/V:2.38 kJ/cm0 0.4 0.8 1.2 1.6 2 2.4 2.8 3.2 3.6 4100200300400500600700900100011001200Time (sec)Temperature(oC)Figure 2.23 Variation in cooling rates with heat input per unit length of weld (EI/V).Reprinted from Lee et al. (58).
decreases the cooling rate (the slope). Kihara et al. (59) showed that thecooling rate decreases with increasing EI/V and preheating. Figure 2.24 showsthat the cooling rate in ESW, which is known to have a very high Q/V, is muchsmaller than that in arc welding (60). The effects of the heat input, weldingspeed, and preheat on the cooling rate and temperature gradient can be illus-trated by considering the following example.Example: Bead-on-plate welding of a thick steel plate is carried out usingGTAW at 200A, 10V, and 2mm/s. Based on Rosenthal’s three-dimensionalequation, calculate the 500°C cooling rates along the x axis of the workpiecefor zero and 250°C preheating.The arc efﬁciency is 70% and the thermal con-ductivity is 35W/m°C.Along the x axis of the workpiece,y = z = 0 and R = x (2.13)Therefore, Equation (2.10) becomes(2.14)Therefore, the temperature gradient is(2.15)From the above equation and(2.16)∂∂xtVTÊËˆ¯=∂∂ ppTxQx xkT TQtÊËˆ¯=-= --( )212202T TQkx- =02p56 HEAT FLOW IN WELDINGElectroslagweldArc weld0 2 4 6 8 10 12 14-1826054081510951370165019250500100015002000250030003500Time, minTemperature,oCTemperature,oFFigure 2.24 Thermal cycles of electroslag and arc welds. Reprinted from Liu et al.(60).
the cooling rate is(2.17)Without preheating the workpiece before welding,(2.18)With 250°C preheating,(2.19)It is clear that the cooling rate is reduced signiﬁcantly by preheating. Pre-heating is a common practice in welding high-strength steels because it reducesthe risk of heat-affected zone cracking. In multiple-pass welding the inter-pass temperature is equivalent to the preheat temperature T0 in single-passwelding.Equation (2.17) shows that the cooling rate decreases with increasing Q/V,and Equation (2.15) shows that the temperature gradient decreases withincreasing Q.2.3.3 Power Density DistributionFigure 2.25 shows the effect of the power density distribution of the heatsource on the weld shape (24). Under the same heat input and welding speed,weld penetration decreases with decreasing power density of the heat source.As an approximation, the power density distribution at the workpiece surfaceis often considered Gaussian, as shown by the following equation:(2.20)where q is the power density, Q the rate of heat transfer from the heat sourceto the workpiece, and a the effective radius of the heat source.2.3.4 Heat Sink Effect of WorkpieceKihara et al. (59) showed that the cooling rate increases with the thickness ofthe workpiece. This is because a thicker workpiece acts as a better heat sinkto cool the weld down. Inagaki and Sekiguchi (61) showed that, under theqQara=-ÈÎÍ˘˚˙33222pexp∂∂pTt xÊËˆ¯= - ¥ ∞ ¥ ¥( )∞ - ∞( )¥ ¥= ∞-2 35 2 10500 2500 7 200 102032W m C m sC CA VC s.∂∂pTt xÊËˆ¯= - ¥ ∞ ¥ ¥( )∞ - ∞( )¥ ¥= ∞-2 35 2 10500 250 7 200 107132W m C m sC CA VC s.∂∂∂∂∂∂pTtTxxtkVT TQx t TÊËˆ¯=ÊËˆ¯ÊËˆ¯= --( )202EFFECT OF WELDING PARAMETERS 57
same heat input and plate thickness, the cooling time is shorter for ﬁlletwelding (a T-joint between two plates) than for bead-on-plate welding becauseof the greater heat sink effect in the former.2.4 WELD THERMAL SIMULATOR2.4.1 The EquipmentThe thermal cycles experienced by the workpiece during welding can be dupli-cated in small specimens convenient for mechanical testing by using a weldthermal simulator called Gleeble, a registered trademark of Dynamic Systems.58 HEAT FLOW IN WELDINGFigure 2.25 Effect of power density distribution on weld shape in GTAW of 3.2-mm6061 aluminum with 880W and 4.23mm/s. From Kou and Le (24).
These simulators evolved from an original device developed by Nippes andSavage in 1949 (62). Figure 2.26 shows a specimen being resistance heated bythe electric current passing through the specimen and the water-cooled jawsholding it (63). A thermocouple spot welded to the middle of the specimen isconnected to a feedback control system that controls the amount of electriccurrent passing through the specimen such that a speciﬁc thermal cycle can beduplicated.2.4.2 ApplicationsThere are many applications for weld thermal simulators. For instance, aweld thermal simulator can be used in conjunction with a high-speeddilatometer to help construct continuous-cooling transformation diagramsuseful for studying phase transformations in welding and heat treating ofsteels.By performing high-speed tensile testing during weld thermal simulation,the elevated-temperature ductility and strength of metals can be evaluated.This is often called the hot-ductility test. Nippes and Savage (64, 65), forinstance, used this test to investigate the heat-affected zone ﬁssuring inaustenitic stainless steels.Charpy impact test specimens can also be prepared from specimens (1 ¥1cm in cross section) subjected to various thermal cycles. This synthetic-specimen or simulated-microstructure technique has been employed bynumerous investigators to study the heat-affected-zone toughness.WELD THERMAL SIMULATOR 59Figure 2.26 A weld simulator specimen held between two water-cooled jaws andresistance heated by electric current passing through it. Courtesy of Dynamic SystemsInc. (63).